Scanning Tunneling Microscopy of Metals and Semiconductors ... · PDF fileScanning Tunneling...
Embed Size (px)
Transcript of Scanning Tunneling Microscopy of Metals and Semiconductors ... · PDF fileScanning Tunneling...
Scanning Tunneling Microscopy of Metals and Semiconductors
Applications of scanning tunneling microscopy (STM) to surfaces of both metals and semiconductors
have rapidly expanded during the last fifteen years. Initial STM studies in both cases focused on
structural imaging as well as measurement of electronic properties using scanning tunneling
spectroscopy (STS). That early work was primarily for low-index surfaces, as reviewed by Hamers
[97H1]. Later studies included a much greater range of surfaces and measurement techniques. The
following literature overview summarizes the STM/STS studies of crystalline surfaces of metals and
semiconductors from 1997 to 2012. The elements and compounds are listed with alphabetical order, and
within each material the topics are ordered from lower to higher index surfaces.
The metal surfaces are rich in physical phenomena and many metallic surfaces are important for
adsorbate ordering, nanostructure formation and surface catalysis processes. The focus of STM studies
on metal surfaces from 1997 to 2012 varies depending on the type of metal surface or surface index. On
some metal surfaces such as Ag(111) and Cu(111), the existence of a two dimensional surface state near
the Fermi level influences adatom diffusion, epitaxial growth, equilibrium crystal shapes,
reconstructions, surface chemical reactions, and adsorbate ordering processes. STM with its imaging
and spectroscopic capabilities is the right choice of instrument to explore the surface state related
phenomena on these surfaces, including the surface state lifetime, surface state electron confinement,
and the electron standing waves. STM is also used to study the image-potential states on metal surfaces.
The ‘z’ versus V spectroscopic data show the existence of Rydberg-like series of potentials along the
surface normal direction on many metal surfaces. The measurements further reveal a strong influence of
Stark effect and tip shape on the observed quantized potentials. The dynamic at step edges are also of
interest because they can influence the crystal growth. Dislocations at surfaces are also vital in many
areas of materials science. For example, screw dislocations can influence the crystal growth, and can
modify surface stress. Detailed STM studies for dislocations have been carried out on Ag(111) and
Au(111) surfaces. On vicinal surfaces such as Au(110), Ag(110), Pt(110) and Ir(110), the surface
roughening and phase transitions are of main interest. The STM measurements are focused on Ising
type phase transition and surface roughening transitions at elevated temperatures. On 5d metals such as
Au, Pt and Ir surfaces, the top most surface layer often reconstruct due to strain. STM studies on
Au(100), Pt(100) and Ir(100) surfaces are mainly devoted to surface reconstruction and related
phenomena. On Au(111) surface, the stability of herringbone type reconstruction has been explored by
forming vacancy islands. Surfaces having spin density of states such as Ni, Cr, and Fe, the interplay
between the spin and local density of state at the surface have been the focus of the studies. The bcc
metal surfaces such as Mo, W, and Ta are important for many applications however, preparation of a
clean and atomically flat surface for STM studies is difficult. Nevertheless, a number of studies have
reported for atomic resolution images on these surfaces as well.
The following literature overview summarizes the STM/STS studies of bulk crystal surfaces of pure
metals. Many STM studies of metal surfaces from 1997 to 2012 are extensions of initial findings that
have been reported prior to this period. This overview does not include bulk and surface metallic alloys,
thin-films, adsorbates, and nanostructures on metallic surfaces.
Atomically resolved STM images show the expected square lattice arrangement of individual atoms on
this surface [06C]. Changes in surface morphology due to ion sputtering process has been investigated
using STM topographic images acquired over different sputter conditions and substrate temperatures
[01C]. The study shows that periodic pattern of square islands are formed on this surface when
sputtering at substrate temperatures between 240 and 440 K.
STM image of Ag(110) acquired at 300K shows the expected structure of atomic rows running along
 surface direction [99K, 00K]. On this surface, the role of tip-surface interaction has been studied
using an elevated temperature STM [00K, 00S2]. At 360K, the step edges of Ag(110) show several nm
long fringes along the scanning direction (Fig. 1) [00K] and this effect is explained as diffusion at step
edges induced by the STM tip. At 300K, however, scanning parallel to the closed-pack direction along
the step edge does not show any fringes, thus stable step edge can be observed in STM images. Other
studies on Ag(110) include the study of surface steps [00B2] and changes in surface morphology due to
ion sputtering processes [97R2, 01C].
Fig. 1. (a and b) 25×25nm2 STM images of the same
area of Ag(110) at 360±10 K and different fast
scanning directions (indicated by arrows) revealing
fringy [ ̅ ] steps that run parallel to the close-packed rows [-25mV, 1.8nA]. (c and d): 25×20 nm2 STM
images of the same area of Ag(110) at 300 K with the
fast scanning direction (indicated by arrows)
perpendicular (c) and parallel (d) to the [ ̅ ] steps. [−257 mV, −0.5 nA]. The insets show the respective
raw data at a higher magnification [00K].
Ag(111) surface has a Shockley-type surface state around -65 meV, which forms two dimensional
nearly free electron gas parallel to the surface and generates many interesting physical phenomena
[97L, 98B, 98L3, 8L4, 98L5, 99L, 02M2, 03V]. The surface state of Ag(111) can be directly
determined by using dI/dV-V spectroscopy, where the surface state onset appears as a rise in dI/dV
signal (Fig. 2) [98L4]. To avoid the influence of defects or step edges, the surface state needs to be
determined at large flat terraces [99L]. During the spectroscopic measurements, the changes in the tip
positions can alter the barrier transmission probability that can in turn change the positions of dI/dV
maxima in the spectroscopic curve. Li et al. [97L] describes a way to correct this by dividing the dI/dV
data with the transmission coefficient T, which is defined as:
Here, t and s are the work functions of the tip and the Ag(111) sample, and , where z0 is the tip height. This procedure is applicable only when the measurements are performed at 1
nm or more distance away from a step edge on Ag(111). From the geometric line width of the rise of
surface state onset in the dI/dV curve (Fig. 2b), the lifetime of surface state electrons can be determined
[98L4, 06B] as well.
These surface state electrons scatter from defects and step edges on Ag(111) and produce
interference patterns known as electron standing waves (Fig. 3). The electron standing waves can be
directly observed even in normal STM images when acquired at lower biases close to the Fermi energy
on Ag(111). At higher biases, however, the tunneling current represents a weighted integral over a
range of energies, and the oscillatory signal is smeared out.
Fig. 2. (a) Surface state of Ag(111) appears as the step-like onset
in the dI/dV spectrum. (b) and (c) show the onset region in detail
from spectra recorded with different tips, showing the variation in
slope above the onset. Vm is the modulation voltage [98L4].
Fig. 3. (a) dI/dV line scan across a Ag(111)
narrow terrace measured as a function of bias
(E), and (b) corresponding model image
Morgenstern et al. [02M2] investigated the confinement of surface state electrons in narrow steps of
Ag(111). Tunneling spectroscopy data taken over different terrace widthes reveal that the surface state
on-set energy is shifted towards the Fermi energy (EF) when the width is decreased (Fig. 4) due to
depopulation of the surface state electrons at narrow terraces. When the terrace width is less than F/2,
where F is the Fermi wavelength of the silver, the electrons can be no longer confined at the terraces
because it switches from the terrace to a step modulation of surface electron wave function [02M2].
Fig. 4. dI/dV spectra
show shifting of the
surface state on-set
towards the Fermi level
when the terrace width is
STM is also used to study surface defects such as dislocations. From an atomically resolved STM
image of a screw dislocation [02C], the in-plane component of the Burgers vector can be measured
(Fig. 5) allowing a direct determination of the Burgers vectors of the individual partial dislocations as
[ ] dissociation on ( ̅ . In contras